© 2012 Jeng and Hwang, licensee InTech. This is an open access chapter distributed under the terms of the
Creative Commons Attribution License (http://creativecommons.org/licenses/by/3.0), which permits
unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Controlling the Alignment of Polyimide
for Liquid Crystal Devices
Shie-Chang Jeng and Shug-June Hwang
Additional information is available at the end of the chapter
Liquid crystal (LC) devices have been popular for use in photonics products, such as
displays for mobile phones, televisions and computers. As shown in Fig. 1, a typical LC
device consists of a thin LC layer sandwiched between a pair of indium tin oxide (ITO)
conducting glass substrates with a cell gap of few micrometers. Polyimide (PI) as a
polymeric material characterized by its outstanding mechanical, thermal and electrical
properties at moderate high temperature has been widely applied in the LC displays (LCDs)
industry as the alignment layers to align LC molecules in a certain orientation and
conformation with a specific pretilt angle, the angle between the director of the LC
molecules and the PI alignment layer. The pretilt angle is very important and required for
LC devices to obtain a defect-free alignment and also to improve their electro-optical
performance, such as driving voltage, response time, color performance and viewing angle.
However, the applications of conventional PIs in LCDs are limited by a small tuning range
of pretilt angle (~ few degrees) either by controlling the rubbing depth or the number of
rubbings (Paek et al., 1998).
Figure 1. The typical structure of a liquid crystal device.
The pretilt angle of an LCD is either near zero degrees or 90 degrees for using the
conventional homogeneous and homeotropic PI materials, respectively. The technique of
PI alignment layer
High Performance Polymers – Polyimides Based – From Chemistry to Applications 88
producing homogeneous and homeotropic PI is mature in the LCDs industry. For example,
the introduction of long alkyl groups into the aromatic diamines has been applied for
increasing the pretilt angle from near zero degrees to near 90 degrees (Tsuda, 2011).
However, the required specific pretilt angles of LCDs depend on their operation modes, for
example, near zero degrees for in-plane switching (displays for iPhone and iPad), several
degrees for the twisted nematic mode (displays for Laptop computers), more than 5° for the
supertwisted nematic mode, 45o ~ 60o for no-bias optically-compensated bend (OCB) mode
(LCDs with fast response time and wide viewing angle) and the bi-stable bend-splay (BBS)
mode (LCDs requiring memory effect, such as e-books), and near 90 degrees for the vertical
alignment mode (LCDs for TVs). Among of them, the OCB LCD has attracted much
attention in recent years due to its fast response time and inherent wide view angle property
(Acosta et al., 2000), and the memory effect of a bistable LCD is highly suitable for
electronic-paper applications due to the low power consumption. The OCB LCD is operated
between the bend state and the homeotropic state. A bias voltage should be applied to
transfer a conventional OCB mode from the initially splay state to the bend state. Using a
high pretilt angle of ~50o is sufficient to provide a stable bend state in an OCB mode at no
bias voltage (Yeung & Kwok, 2006a), and it has been successfully demonstrated to reach the
no-bias OCB operation. In general, an alignment layer with a high pretilt angle of around
45o ~ 58o is required for a BBS LCD providing the same splay and bend deformation energies
(Yu & Kwok, 2004); therefore bistability between bend and splay states are reached.
In order to obtain a demanded pretilt angle for different LCD applications, there are many
methods have been developed in the last two decades for controlling the pretilt angle of LC
with a wide range, such as: obliquely-evaporated silicon monoxide (Uchida et al., 1980;
Janning, 1992), polymer-stabilized alignment (Chen & Chu, 2008), hybrid mixture of two
materials (Yeung et al., 2006b; Vaughn et al., 2007; Wu et al., 2008; Ahn et al., 2009), nano-
structured surfaces (Komitov, 2008), chemical synthesis (Nishikawa, 2000; Tsuda, 2011), and
stacked PI alignment layers (Lee et al., 2009). However, the reliability, the mass production
capability and ease of material synthesis for those developed techniques are questionable.
For example, the complicate molecular design and synthetic processes are required for a
new development of alignment material.
Recently, we have developed a new approach to align LC vertically by adding polyhedral
oligomeric silsesquioxane (POSS) nanoparticles in LCDs (Jeng et al., 2007; Hwang et al.,
2009). POSS nanoparticles with nano-sized cage structures have been incorporated into
polymers for improving their thermal, mechanical and oxidation resistance (Xiao et al., 2003;
Yei et al., 2004). A typical structure of the POSS molecule is shown in Fig. 2, with R
indicating the functional group (Sigma-Aldrich Corp., St. Louis, MO, USA). In our recent
work, we have demonstrated that the pretilt angle of LC molecules can be continuously
controlled by using conventional homogeneous PI alignment material doped with different
concentrations of POSS nanoparticles (Hwang et al. 2010). The addition of POSS in the
homogenous PI decreases the surface energy of the PI alignment layer and generates the
controllable pretilt angle θp in a range of 0°
Controlling the Alignment of Polyimide for Liquid Crystals Devices 89
The pretilt angle of a PI alignment layer can also be controlled by ultra-violet (UV)
irradiation (Lu et al., 1996; Yoshida & Koike, 1997; Ichimura, 2000; Chigrinov et al., 2008).
UV irradiation on PI alignment films can produce extensive physical and chemical changes,
such as photo-isomerization, photo-dimerization and photo-decomposition (Ichimura, 2000;
Chigrinov et al., 2008), for PI materials with or without photo-functional groups. Techniques
of photo-alignment by polarized and non-polarized UVs had been developed in the 90s and
have recently matured for producing large LCDs (Miyachi et al., 2010). UV-modified PI
films have also been applied for fabricating LC photonics devices, such as single-cell-gap
transflective LCDs and LC Fresnel lens (LCFL) recently (Fan et al., 2004; Jeng et al., 2010;
Hwang et al. 2012). The required pretilt angle can be achieved by using UV irradiation for
controlling the surface energy of a PI film. Therefore, any LC device requiring patterned
alignment areas with different pretilt angles can be obtained by this method.
Figure 2. The structure of a PSS-(3-(2-Aminoethyl)amino)propyl-Heptaisobutyl substituted POSS
nanoparticle (Sigma-Aldrich Corp., St. Louis, MO, USA).
In this chapter, we reported our developed non-synthetic techniques for controlling the
pretilt angles of LC molecules either by doping homogeneous PI with POSS nanoparticles or
treating homeotropic PI with UV. The surface energy of POSS-doped PI and UV-treated PI
alignment layers were studied to investigate the mechanism of pretilt control. The LC
devices, such as no-bias OCB LCDs, LC Fresnel lenses and LC phase gratings, were
fabricated and presented in this chapter.
2. Sample preparation
2.1. POSS-doped polyimide
Several commercial homogeneous PI materials from Chimei, Daily Polymer and Nissan
Chemical have been tried in the experiments, and some of them work. The POSS
nanoparticle, PSS-(3-(2-Aminoethyl)amino)propyl-Heptaisobutyl substituted POSS
(SIGMA-ALDRICH) as shown in Fig. 2, was purchased and used in the experiment without
further treatment and purification. A powerful ultrasonic processor (S4000, Misonix) for
producing the mixture of the POSS/PI was applied for obtaining a good dispersion of 0.2
wt% POSS doped in PI. The mixture was then filtered through a 200 nm syringe filter. The
High Performance Polymers – Polyimides Based – From Chemistry to Applications 90
mixture was further diluted with pure PI in order to generate different concentration of
POSS in PI. The POSS/PI films were cast on ITO conducting glass substrates by spin coating
at 1000 rpm for 5 s and at 4000 rpm for 60 s. They were then prebaked at 100 oC for 10
minutes and post-baked at 180 oC for 4 hours in a vacuum oven to cure the POSS/PI mixture
for forming the alignment layers. The manufacture parameters used here may depend on
the PI materials. The surface of the PI alignment layer was then mechanically buffed by
using a nylon cloth in such a way that the alignment layer was rubbed once in each
direction. Prior to film casting, the ITO glass substrates were cleaned with distilled water,
2-propanol and acetone in an ultrasonic bath and dried at 80 °C for 1 hr.
2.2. UV-treated polyimide
Several commercial homeotropic PI materials from Chimei and JSR have been tried in the
experiments, and they required different curing parameters of UV dosage. As shown in Fig.
3, the homeotropic PIs were first spin-coated on the ITO substrates in order to fabricate the
UV-treated PI alignment layer. Then, they were pre-baked at 80°C for 10 minutes and post-
baked at 210°C for 35 minutes in a vacuum oven. Subsequently, an UV light irradiated the
homeotropic PI film through a designed photo mask. For those LC devices requiring
precision alignment patterns, the substrates were laminated before UV irradiation as shown
in Fig. 3. After finishing UV irradiati